## Ultra-high-*Q* three-dimensional photonic crystal nano-resonators

Optics Express, Vol. 15, Issue 25, pp. 17254-17263 (2007)

http://dx.doi.org/10.1364/OE.15.017254

Acrobat PDF (700 KB)

### Abstract

Two nano-resonator modes are designed in a woodpile three-dimensional photonic crystal by the modulation of unit cell size along a low-loss optical waveguide. One is a dipole mode with 2.88 cubic half-wavelengths mode volume. The other is a quadrupole mode with 8.3 cubic half-wavelengths mode volume. Light is three-dimensionally confined by a complete photonic band gap so that, in the analyzed range, the quality factor exponentially increases as the increase in the number of unit cells used for confinement of light.

© 2007 Optical Society of America

## 1. Introduction

1. E. Yablonovitch, “Inhibited Spontaneous Emission in Solid-State Physics and Electronics,” Phys. Rev. Lett. **58**, 2059 (1987). [CrossRef] [PubMed]

2. S. John, “Strong Localization of Photons in Certian Disordered Dielectric Superlattices,” Phys. Rev. Lett. **58**, 2486 (1987). [CrossRef] [PubMed]

*V*) is kept to be small, the quality factor (

*Q*) can be infinitely large for a passive, infinitely-large photonic crystal nano-resonator in a complete photonic band gap. Therefore, actual

*Q*factors would be limited by other loss mechanisms, including the material absorption and the fabrication inaccuracy. In the photonic crystal community, the

*Q*factor exceeding one million is often recognized as an ultra-high-

*Q*while 100 millions or greater is typically considered to be an ultra-high-

*Q*in the microcavity community. Ultra-high-

*Q*nano-resonator modes [3

3. E. Kuramochi, M. Notomi, S. Mitsugi, A. Shinya, T. Tanabe, and T. Watanabe, “Ultrahigh-Q photonic crystal nanocavities realized by the local width modulation of a line defect,” Appl. Phys. Lett. **88**, 041112 (2006). [CrossRef]

4. B.-S. Song, S. Noda, T. Asano, and Y. Akahane, “Ultra-high-Q photonic double-heterostructure nanocavity,” Nature Materials **4**, 207–210 (2005). [CrossRef]

5. T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H. M. Gibbs, G. Rupper, C. Ell, O. B. Shchekin, and D. G. Deppe, “Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity,” Nature **432**, 200–203 (2004). [CrossRef] [PubMed]

6. M. Notomi, A. Shinya, S. Mitsugi, G. Kira, E. Kuramochi, and T. Tanabe, “Optical bistable switching action of Si high-Q photonic-crystal nanocavities,” Opt. Express **13**, 2678–2687 (2005). [CrossRef] [PubMed]

8. T. J. Kippenberg, S. M. Spillane, and K. J. Vahala, “Kerr-Nonlinearity Optical Parametric Oscillation in an Ultrahigh-Q Toroid Microcavity,” Phys. Rev. Lett. **93**, 083904 (2004). [CrossRef] [PubMed]

9. T. Baba, T. Hamano, F. Koyama, and K. Iga, “Spontaneous emission factor of a microcavity DBR surface-emitting laser,” IEEE J. of Quantum Electron. **27**, 1347–1358 (1991). [CrossRef]

10. H. Mabuchi and A. C. Doherty, “Cavity Quantum Electrodynamics: Coherence in Context,” Science **298**, 1372–1377 (2002). [CrossRef] [PubMed]

11. K. J. Vahala, “Optical microcavities,” Nature **424**, 839–846 (2003). [CrossRef] [PubMed]

*g/κ*∝

*Q*/√

*V*and

*g*/

*γ*∝1/√

*V*are desired for improving the quantum coherence, where

*g*is the emitter-cavity field coupling rate, and κ and

*γ*are decay rates of cavity and emitter. Vacuum Rabi splitting was observed between a single quantum dot (SQD) and a compact resonator [5

5. T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H. M. Gibbs, G. Rupper, C. Ell, O. B. Shchekin, and D. G. Deppe, “Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity,” Nature **432**, 200–203 (2004). [CrossRef] [PubMed]

12. J. P. Reithmaier, G. Sek, A. Loffler, C. Hofmann, S. Kuhn, S. Reitzenstein, L. V. Keldysh, V. D. Kulakovskii, T. L. Reinecke, and A. Forchel, “Strong coupling in a single quantum dot-semiconductor microcavity system,” Nature **432**, 197–200 (2004). [CrossRef] [PubMed]

13. E. Peter, P. Senellart, D. Martrou, A. Lemaitre, J. Hours, J. M. Gerard, and J. Bloch, “Exciton-Photon Strong-Coupling Regime for a Single Quantum Dot Embedded in a Microcavity,” Phys. Rev. Lett. **95**, 067401 (2005). [CrossRef] [PubMed]

5. T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H. M. Gibbs, G. Rupper, C. Ell, O. B. Shchekin, and D. G. Deppe, “Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity,” Nature **432**, 200–203 (2004). [CrossRef] [PubMed]

7. S. M. Spillane, T. J. Kippenberg, and K. J. Vahala, “Ultralow-threshold Raman laser using a spherical dielectric microcavity,” Nature **415**, 621–623 (2002). [CrossRef] [PubMed]

8. T. J. Kippenberg, S. M. Spillane, and K. J. Vahala, “Kerr-Nonlinearity Optical Parametric Oscillation in an Ultrahigh-Q Toroid Microcavity,” Phys. Rev. Lett. **93**, 083904 (2004). [CrossRef] [PubMed]

6. M. Notomi, A. Shinya, S. Mitsugi, G. Kira, E. Kuramochi, and T. Tanabe, “Optical bistable switching action of Si high-Q photonic-crystal nanocavities,” Opt. Express **13**, 2678–2687 (2005). [CrossRef] [PubMed]

*V/Q*

^{2}. A two-dimensional (2D) photonic crystal slab cavity [14

14. O. Painter, R. K. Lee, A. Scherer, A. Yariv, J. D. O’Brien, P. D. Dapkus, and I. Kim, “Two-Dimensional Photonic Band-Gap Defect Mode Laser,” Science **284**, 1819–1821 (1999). [CrossRef] [PubMed]

*Q*factor is limited and saturates even for a structure with an infinite number of layers. Many designs [3

3. E. Kuramochi, M. Notomi, S. Mitsugi, A. Shinya, T. Tanabe, and T. Watanabe, “Ultrahigh-Q photonic crystal nanocavities realized by the local width modulation of a line defect,” Appl. Phys. Lett. **88**, 041112 (2006). [CrossRef]

4. B.-S. Song, S. Noda, T. Asano, and Y. Akahane, “Ultra-high-Q photonic double-heterostructure nanocavity,” Nature Materials **4**, 207–210 (2005). [CrossRef]

15. K. Srinivasan and O. Painter, “Momentum space design of high-Q photonic crystal optical devices”, Opt. Express **10**, 670–684 (2002). [PubMed]

18. D. Englund, I. Fushman, and J. Vuckovic, “General recipe for designing photonic crystal cavities,” Opt. Express **13**, 5961–5975 (2005). [CrossRef] [PubMed]

*Q*factor of 7×10

^{7}has been reported for

*V*~12 (λ

_{0}/2

*n*)

^{3}in their modeling [3

3. E. Kuramochi, M. Notomi, S. Mitsugi, A. Shinya, T. Tanabe, and T. Watanabe, “Ultrahigh-Q photonic crystal nanocavities realized by the local width modulation of a line defect,” Appl. Phys. Lett. **88**, 041112 (2006). [CrossRef]

_{0}and

*n*are the wavelength of light in vacuum and the refractive index in a maximum field position. However, the

*Q*factor increases at a price of a larger mode volume [18

18. D. Englund, I. Fushman, and J. Vuckovic, “General recipe for designing photonic crystal cavities,” Opt. Express **13**, 5961–5975 (2005). [CrossRef] [PubMed]

*et al*[17

17. Z. Zhang and M. Qiu, “Small-volume waveguide-section high Q microcavities in 2D photonic crystal slabs”, Opt. Express **12**, 3988–3995 (2004). [CrossRef] [PubMed]

*Q*factor of 10

^{5}for 2.3 (λ

_{0}/2

*n*)

^{3}mode volume. It is still a challenge to build ultra-high-

*Q*resonators as a mode volume approaches (λ

_{0}/2

*n*)

^{3}. A complete photonic band gap may resolve this challenge. Three-dimensional photonic crystal nano-cavity modes may be constructed in a complete photonic band gap, so ultra-high

*Q*factors can be obtained even at a small mode volume. The

*Q*factor might not become a factor limiting the figure of merit for each application. In addition, the investigation of light localization in a complete photonic band gap would be insightful for understanding the fundamental limits in light localization.

19. S. Noda, K. Tomoda, N. Yamamoto, and A. Chutinan, “Full Three-Dimensional Photonic Bandgap Crystals at Near-Infrared Wavelengths,” Science **289**, 604–606 (2000). [CrossRef] [PubMed]

20. M. Qi, E. Lidorikis, P. T. Rakich, S. G. Johnson, J. D. Joannopoulos, E. P. Ippen, and H. I. Smith, “A three-dimensional optical photonic crystal with designed point defects,” Nature **429**, 538–542 (2004). [CrossRef] [PubMed]

21. S. Ogawa, M. Imada, S. Yoshimoto, M. Okano, and S. Noda, “Control of Ligth Emission by 3D Photonic Crystals,” Science **305**, 227–229 (2004). [CrossRef] [PubMed]

22. M. Okano, A. Chutinan, and S. Noda, “Analysis and design of single-defect cavities in a three-dimensional photonic crystal,” Phys. Rev. B **66**, 165211 (2002). [CrossRef]

24. M. Okano and S. Noda, “Analysis of multimode point-defect cavities in three-dimensional photonic crystals using group theory in frequency and time domains,” Phys. Rev. B **70**, 125105 (2004). [CrossRef]

*Q*3D photonic crystal nano-resonators consisting of straight rods only. We confirm that ultra-high

*Q*factors can be obtained at a small mode volume, and they will not saturate in the range analyzed. In 2D photonic crystal slab geometries, the double-heterostructure designs achieved the

*Q*factors exceeding one million, and this concept is applied to construct 3D photonic crystal nano-cavities in this work. We use a layered woodpile structure [25

25. K. M. Ho, C. T. Chan, C. M. Soukoulis, R. Biswas, and M. Sigalas, “Photonic band gaps in three dimensions: new layer-by-layer periodic structures,” Solid State Communications **89**, 413–416 (1994). [CrossRef]

26. S. Kawashima, L. H. Lee, M. Okano, M. Imada, and S. Noda, “Design of donor-type line-defect waveguides in three-dimensional photonic crystals,” Opt. Express **13**, 9774–9781 (2005). [CrossRef] [PubMed]

*Q*3D photonic crystal nano-resonators in a complete photonic band gap by using the modulation of unit cell size.

## 2. Method

27. S. Johnson and J. Joannopoulos, “Block-iterative frequency-domain methods for Maxwell’s equations in a planewave basis,” Opt. Express **8**, 173–190 (2001). [CrossRef] [PubMed]

28. A. Farjadpour, D. Roundy, A. Rodriguez, M. Ibanescu, P. Bermel, J. D. Joannopoulos, S. G. Johnson, and G. Burr, “Improving accuracy by subpixel smoothing in FDTD,” Opt. Lett. **31**, 2972–2974 (2006). [CrossRef] [PubMed]

^{5}plane waves are used for dispersion calculation. Three-dimensional FDTD is then used to calculate resonant frequencies and

*Q*factors, and to visualize field profiles of the cavity modes. Mode volumes are calculated by the definition given n by

*V*=∫∫∫

*ε*(

*r*̄)|

*E*(

*r*̄)|

^{2}

*dV*/max[

*ε*(

*r*̄)|

*E*|

^{2}]. The perfect matching layer (PML) boundary condition [29

29. J.-P. Berenger, “A Perfectly Matched Layer for the Absorption of Electromagnetic Waves,” J. Comput. Phys. **114**, 185–200 (1994). [CrossRef]

*N*×1×

*N*unit cells, where

*N*is an integer number. In all calculations, the resolution is 30 points per lattice constant, corresponding to approximately 75 points per wavelength.

*w/a*and

*h/a*are set to 0.3, where

*w*is the width of each rod in xy plane,

*h*is the height in z direction, and

*a*is the center-to-center distance of the rods in the same layer, also known as a unit cell length in x and y directions. The unit cell volume is

*a*×

*a*×

*a*, where

_{z}*a*=4

_{z}*h*is the unit cell length in z direction. The frequency in this work is represented by a normalized frequency

*a*/λ

_{0}. For a woodpile unit cell with the parameters above, the complete photonic band gap ranges from 0.3526 to 0.4252.

*N*and

_{x}, N_{y}*N*stand for the total number of unit cells in each direction.

_{z}## 3. Results and discussion

26. S. Kawashima, L. H. Lee, M. Okano, M. Imada, and S. Noda, “Design of donor-type line-defect waveguides in three-dimensional photonic crystals,” Opt. Express **13**, 9774–9781 (2005). [CrossRef] [PubMed]

*wx*, and y direction is defined as the propagation direction. Fig. 1(b) illustrates the dispersion relation of each guiding mode inside the complete photonic band gap for

*wx/a*=0.6. Note that there is a mode gap region in which no modes exist between the forth (mode-b) and the fifth lowest mode (mode-c) within the bandgap. In this frequency range, light propagation is not allowed in any direction. There is another large mode gap below the mode-a. The width and position of the mode gaps change when the width of the line defect is varied, and our modeling results are summarized in Fig. 1(c). The mode gaps also shift when the unit cell is distorted or the rod width is varied along the light propagation direction. In order to construct resonators, we use two types of waveguides with different unit cell length or rod width in waveguide direction, but both have the same unit cells in xz directions. The unit cell sizes are

*a*×

*a*×

*a*in waveguide I, and

_{z}*a*×

*a*

^{′}×

*a*in waveguide II. A double heterostructure is constructed by sandwiching waveguide II with two waveguide I geometries, and the central waveguide II has only one unit cell in y direction as shown in Fig. 2. The lattice matching condition is satisfied because the unit cells in these two types of waveguides are same in xz plane. If a guiding mode of the waveguide II is inside a mode gap of the waveguide I, the mode defined by the waveguide II cannot propagate into waveguide I region, and thus a resonator is formed in a complete photonic band gap. The waveguide II is seen as a core region and the waveguide I is considered as a cladding region.

_{z}*Q*factor of the waveguide mode-a with defect width

*w*=0.6, and that of the mode-c in a waveguide with

_{x}/a*w*=0.7, assuming an infinite number of unit cells along the waveguide direction; see Fig. 1(d). The analyzed supercell size is (

_{x}/a*Na*×

*a*×

*Na*) for each point, where

_{z}*N*is a positive, integer number of unit cells along x and z directions. The

*Q*factor exponentially increases as

*N*increases. This waveguide mode would also be useful as a low-loss optical waveguide. In the analyzed N range, the

*Q*factor of the mode-a is about one order of magnitude higher than that of the mode-c, which means the power losses toward x and z directions are relatively small for the mode-a. The slope of the

*Q*-factor increase is steeper for the

*w*=0.7 waveguide than that for the

_{x}/a*w*=0.6 because the mode is close to a midgap point.

_{x}/a*w*=0.7 waveguide (WG0.7) and pull the mode-c into the mode gap B by increasing the unit cell length and the rod width of the waveguide II along the waveguide direction. We induce a small amount of unit-cell-length modulation in order to preserve the waveguide mode and also observe the transition from loose confinement to tight confinement of light. At first, the unit cell length

_{x}/a*a*

^{’}is increased to 1.033

*a*, and the rod width in the core region remains the same. One mode is found at

*a/λ*

_{0}=0.3928. It has a similar field distribution as in the waveguide (Fig. 3(a)), but due to the mode gap effect, the field decays in the cladding waveguide region; see Fig. 3(b). The resonant frequency is very close to an upper edge of the mode gap B. As a result, the mode can still be coupled to the guided mode in the cladding waveguide, and the field distribution is elongated along y direction. The

*Q*factor does not increase rapidly as the number of unit cells increases.

*a*

^{′}=1.067

*a*, and width

*w*

_{y}^{′}=0.333

*a*. This way, a mode with lower resonant frequency

*a*/

*λ*

_{0}=0.3898 is formed. The mode frequency is located at the middle of the mode gap (

*a*/λ

_{0}=0.3886). The field profile becomes localized in the center region (Fig. 3(c)), and it appears to be unchanged as the increase in the number of unit cells in the cladding regions. The

*Q*value is calculated for each photonic crystal structure size as shown in Fig. 3(d). In order to evaluate the confinement of light in each direction, we calculate the power loss in each direction. For this mode, the confinement of light per one unit cell is weak along the waveguide direction. When the numbers of cladding layers in x and z directions are fixed at

*N*=7, the

_{x}=N_{z}*Q*factor first grows exponentially as

*N*increases, and then becomes saturated when

_{y}*N*≥23. The confinement of light in y direction becomes strong and, instead, power losses in x and z directions become dominant. Therefore, in order to increase the

_{y}*Q*factor further, we need to increase

*N*and

_{x}*N*. This was confirmed in our modeling. The Q factor saturates around 8486 even with 35 unit cells in y direction if

_{z}*N*and

_{x}*N*are not increased, but increases from 6,974 to 31,941 by adding four more unit cells in x direction and two more in z direction. The modeling results also show that the saturated

_{z}*Q*factor, for constant

*N*and

_{x}*N*values, is close to the waveguide

_{z}*Q*factor for the same

*N*and

_{x}*N*. Waveguide

_{z}*Q*factors are calculated by neglecting power losses along light propagation direction. The perturbation in the photonic crystal is so small that the losses toward directions normal to the waveguide geometry are considered to remain unchanged. Thus, the cavity

*Q*factor approaches the waveguide

*Q*factor. This way, we can estimate the maximum

*Q*factor that can be reached for certain

*N*and

_{x}*N*values.

_{z}_{0}/2

*n*)

^{3}, which is similar or slightly smaller than typical one for 2D photonic crystal slab double-heterostructure nano-cavities [4

4. B.-S. Song, S. Noda, T. Asano, and Y. Akahane, “Ultra-high-Q photonic double-heterostructure nanocavity,” Nature Materials **4**, 207–210 (2005). [CrossRef]

*Q*factors than others, indicating small power losses in x and z directions. As a result, we would not need a large photonic crystal to obtain an ultra-high

*Q*factor.

*w*=0.6 is used, and the parameters in the core region are:

_{x}/a*a*

^{’}/

*a*=1.2, and

*w*

_{y}^{’}/

*a*=0.4. The mode frequency is 0.3800. The confinement of light per one unit cell is estimated to be very similar for all directions, so we equally increase the unit cell numbers in all directions (

*N*=

_{x}*N*=

_{y}*N*=

_{z}*N*). The

*Q*factor is calculated for each

*N*; see Fig. 6 (b). It increases exponentially with

*N*, and no sign of saturation is observed. In the modeled range, the Q factor can be approximated by the following equation:

*Q*=10

^{1.5214+0.4201N}. We notice that the computational error grows for a structure with a large number of unit cells. The error becomes significant when

*N*is increased to more than 17. The precise evaluation of ultra-high

*Q*factor requires large computational resource. However, we are still able to obtain the

*Q*factor of 2.9×10

^{8}for

*N*=17, and the

*Q*factor is confirmed to significantly increase.

_{0}/2

*n*)

^{3}.

*Q*factor and mode volume with the extent of the modulation. The waveguide with

*w*=0.5 is used because it has the largest mode gap A, which ranges from 0.3576 to 0.4035, in the defect width range analyzed. As the unit cell modulation increases gradually, the resonant frequency decreases as expected (Fig. 7). The Q factor is high for the modes located deep inside the mode gap, and decreases quickly as the mode frequency become close to one of mode gap edges. Modes formed by small modulation, as explained above, can still be coupled to the cladding waveguide, so the loss along the waveguide direction is dominant. The mode is elongated, and the mode volume is large as we can see for the mode with resonant frequency of 0.4028 in Fig. 7. As the mode frequency decreases, the coupling to the cladding waveguide also decreases, and the mode becomes well confined in a small mode volume. For large modulation, the mode is near the lower edge of the mode gap, the

_{x}/a*Q*factor deceases for three possible reasons. First, the coupling to the lower propagation bands in the cladding waveguide might increase. Secondly, the mode is also close to the lower edge of the complete band gap, so the loss in the vertical direction of the waveguide might increase. Thirdly, the unit cells in the core region are significantly distorted, so the losses into the x and z directions in the core region might also grow. Except for the highest frequency mode, all the other modes have very similar mode volume, which is about 3 (λ

_{0}/2

*n*)

^{3}. The volume of higher

*Q*factor modes is slightly larger than that of the modes with lower

*Q*factor.

*Q*nano-resonator modes are designed. The one with 2.88 (λ

_{0}/2

*n*)

^{3}mode volume is pulled down into a middle of a wide mode gap so that it has a steeper slope of the

*Q*factor per one unit cell increment than the other mode. Our study shows that, for the double heterostructure cavity design, the properties of waveguide modes and the mode gap value appear to be determinant factors. It appears to be essential to study low-loss 3D photonic crystal waveguides with a large mode gap inside a complete photonic band gap for tight 3D confinement of light. The designed resonator geometries are unique in that only straight rods are needed. We are working on the fabrication and testing to evaluate the

*Q*factors.

## 4. Conclusion

*Q*nano-resonators with the mode volume close to the fundamental mode. Three-dimensional photonic crystal nanocavities based on unit cell modulation along an optical waveguide are modeled. The calculated

*Q*factors and electromagnetic field profiles indicate that the properties of the cavity modes strongly depend upon original waveguide modes and mode-gap differences between the core and cladding regions. Compact, ultra-high-

*Q*modes are confirmed in our calculation. The modeling results confirm that the

*Q*factor increases exponentially with the number of unit cells in the range analyzed. In the cavity mode induced from a low-loss waveguide mode into the lower wide mode gap in the waveguide with defect width

*w*=0.6, ultra-high

_{x}/a*Q*factors are obtained with a small photonic crystal volume, and the mode volume is as small as 2.88 (λ

_{0}/2

*n*)

^{3}. Photonic crystal volumes required for the

*Q*of one million are approximately 11

^{3}a

^{2}a

_{z}=1331a2az and 11×35×9a

^{2}a

_{z}=3465a

^{2}a

_{z}for the designed dipole and quadrupole modes, respectively, where a2az is one unit cell volume of the cladding region. As expected, 3D photonic crystal cavities formed in a complete band gap are extremely low-loss even for a small mode-volume mode. These designs would be useful for improving the performance in many applications such as the improvement of the quantum coherence in cavity-QED experiments, the reduction of optical switching energy, and the reduction of threshold in lasers such as Raman lasers. For example, the interaction rate for a strong-coupling cavity-QED system would still be increased, and the photon decay rate could be minimized.

## Acknowledgements

## References and Links

1. | E. Yablonovitch, “Inhibited Spontaneous Emission in Solid-State Physics and Electronics,” Phys. Rev. Lett. |

2. | S. John, “Strong Localization of Photons in Certian Disordered Dielectric Superlattices,” Phys. Rev. Lett. |

3. | E. Kuramochi, M. Notomi, S. Mitsugi, A. Shinya, T. Tanabe, and T. Watanabe, “Ultrahigh-Q photonic crystal nanocavities realized by the local width modulation of a line defect,” Appl. Phys. Lett. |

4. | B.-S. Song, S. Noda, T. Asano, and Y. Akahane, “Ultra-high-Q photonic double-heterostructure nanocavity,” Nature Materials |

5. | T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H. M. Gibbs, G. Rupper, C. Ell, O. B. Shchekin, and D. G. Deppe, “Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity,” Nature |

6. | M. Notomi, A. Shinya, S. Mitsugi, G. Kira, E. Kuramochi, and T. Tanabe, “Optical bistable switching action of Si high-Q photonic-crystal nanocavities,” Opt. Express |

7. | S. M. Spillane, T. J. Kippenberg, and K. J. Vahala, “Ultralow-threshold Raman laser using a spherical dielectric microcavity,” Nature |

8. | T. J. Kippenberg, S. M. Spillane, and K. J. Vahala, “Kerr-Nonlinearity Optical Parametric Oscillation in an Ultrahigh-Q Toroid Microcavity,” Phys. Rev. Lett. |

9. | T. Baba, T. Hamano, F. Koyama, and K. Iga, “Spontaneous emission factor of a microcavity DBR surface-emitting laser,” IEEE J. of Quantum Electron. |

10. | H. Mabuchi and A. C. Doherty, “Cavity Quantum Electrodynamics: Coherence in Context,” Science |

11. | K. J. Vahala, “Optical microcavities,” Nature |

12. | J. P. Reithmaier, G. Sek, A. Loffler, C. Hofmann, S. Kuhn, S. Reitzenstein, L. V. Keldysh, V. D. Kulakovskii, T. L. Reinecke, and A. Forchel, “Strong coupling in a single quantum dot-semiconductor microcavity system,” Nature |

13. | E. Peter, P. Senellart, D. Martrou, A. Lemaitre, J. Hours, J. M. Gerard, and J. Bloch, “Exciton-Photon Strong-Coupling Regime for a Single Quantum Dot Embedded in a Microcavity,” Phys. Rev. Lett. |

14. | O. Painter, R. K. Lee, A. Scherer, A. Yariv, J. D. O’Brien, P. D. Dapkus, and I. Kim, “Two-Dimensional Photonic Band-Gap Defect Mode Laser,” Science |

15. | K. Srinivasan and O. Painter, “Momentum space design of high-Q photonic crystal optical devices”, Opt. Express |

16. | J. Vuckovic, M. Loncar, H. Mabuchi, and A. Scherer, “Optimization of the Q factor in photonic crystal microcavities”, IEEE J. of Quantum Electron. |

17. | Z. Zhang and M. Qiu, “Small-volume waveguide-section high Q microcavities in 2D photonic crystal slabs”, Opt. Express |

18. | D. Englund, I. Fushman, and J. Vuckovic, “General recipe for designing photonic crystal cavities,” Opt. Express |

19. | S. Noda, K. Tomoda, N. Yamamoto, and A. Chutinan, “Full Three-Dimensional Photonic Bandgap Crystals at Near-Infrared Wavelengths,” Science |

20. | M. Qi, E. Lidorikis, P. T. Rakich, S. G. Johnson, J. D. Joannopoulos, E. P. Ippen, and H. I. Smith, “A three-dimensional optical photonic crystal with designed point defects,” Nature |

21. | S. Ogawa, M. Imada, S. Yoshimoto, M. Okano, and S. Noda, “Control of Ligth Emission by 3D Photonic Crystals,” Science |

22. | M. Okano, A. Chutinan, and S. Noda, “Analysis and design of single-defect cavities in a three-dimensional photonic crystal,” Phys. Rev. B |

23. | M. Okano, S. Kako, and S. Noda, “Coupling between a point-defect cavity and a line-defect waveguide in three-dimensional photonic crystal,” Phys. Rev. B |

24. | M. Okano and S. Noda, “Analysis of multimode point-defect cavities in three-dimensional photonic crystals using group theory in frequency and time domains,” Phys. Rev. B |

25. | K. M. Ho, C. T. Chan, C. M. Soukoulis, R. Biswas, and M. Sigalas, “Photonic band gaps in three dimensions: new layer-by-layer periodic structures,” Solid State Communications |

26. | S. Kawashima, L. H. Lee, M. Okano, M. Imada, and S. Noda, “Design of donor-type line-defect waveguides in three-dimensional photonic crystals,” Opt. Express |

27. | S. Johnson and J. Joannopoulos, “Block-iterative frequency-domain methods for Maxwell’s equations in a planewave basis,” Opt. Express |

28. | A. Farjadpour, D. Roundy, A. Rodriguez, M. Ibanescu, P. Bermel, J. D. Joannopoulos, S. G. Johnson, and G. Burr, “Improving accuracy by subpixel smoothing in FDTD,” Opt. Lett. |

29. | J.-P. Berenger, “A Perfectly Matched Layer for the Absorption of Electromagnetic Waves,” J. Comput. Phys. |

**OCIS Codes**

(140.3460) Lasers and laser optics : Lasers

(190.0190) Nonlinear optics : Nonlinear optics

(230.5750) Optical devices : Resonators

(270.5580) Quantum optics : Quantum electrodynamics

(140.3945) Lasers and laser optics : Microcavities

**ToC Category:**

Photonic Crystal Cavities

**History**

Original Manuscript: September 27, 2007

Revised Manuscript: November 9, 2007

Manuscript Accepted: November 16, 2007

Published: December 10, 2007

**Virtual Issues**

Physics and Applications of Microresonators (2007) *Optics Express*

**Citation**

Lingling Tang and Tomoyuki Yoshie, "Ultra-high-Q three-dimensional photonic crystal nano-resonators," Opt. Express **15**, 17254-17263 (2007)

http://www.opticsinfobase.org/oe/abstract.cfm?URI=oe-15-25-17254

Sort: Year | Journal | Reset

### References

- E. Yablonovitch, "Inhibited Spontaneous Emission in Solid-State Physics and Electronics," Phys. Rev. Lett. 58, 2059 (1987). [CrossRef] [PubMed]
- S. John, "Strong Localization of Photons in Certian Disordered Dielectric Superlattices," Phys. Rev. Lett. 58, 2486 (1987). [CrossRef] [PubMed]
- E. Kuramochi, M. Notomi, S. Mitsugi, A. Shinya, T. Tanabe, and T. Watanabe, "Ultrahigh-Q photonic crystal nanocavities realized by the local width modulation of a line defect," Appl. Phys. Lett. 88, 041112 (2006). [CrossRef]
- B.-S. Song, S. Noda, T. Asano, and Y. Akahane, "Ultra-high-Q photonic double-heterostructure nanocavity," Nature Materials 4, 207-210 (2005). [CrossRef]
- T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H. M. Gibbs, G. Rupper, C. Ell, O. B. Shchekin, and D. G. Deppe, "Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity," Nature 432, 200-203 (2004). [CrossRef] [PubMed]
- M. Notomi, A. Shinya, S. Mitsugi, G. Kira, E. Kuramochi, and T. Tanabe, "Optical bistable switching action of Si high-Q photonic-crystal nanocavities," Opt. Express 13, 2678-2687 (2005). [CrossRef] [PubMed]
- S. M. Spillane, T. J. Kippenberg, and K. J. Vahala, "Ultralow-threshold Raman laser using a spherical dielectric microcavity," Nature 415, 621-623 (2002). [CrossRef] [PubMed]
- T. J. Kippenberg, S. M. Spillane, and K. J. Vahala, "Kerr-Nonlinearity Optical Parametric Oscillation in an Ultrahigh-Q Toroid Microcavity," Phys. Rev. Lett. 93, 083904 (2004). [CrossRef] [PubMed]
- T. Baba, T. Hamano, F. Koyama, and K. Iga, "Spontaneous emission factor of a microcavity DBR surface-emitting laser," IEEE J. of Quantum Electron. 27, 1347-1358 (1991). [CrossRef]
- H. Mabuchi, and A. C. Doherty, "Cavity Quantum Electrodynamics: Coherence in Context," Science 298, 1372-1377 (2002). [CrossRef] [PubMed]
- K. J. Vahala, "Optical microcavities," Nature 424, 839-846 (2003). [CrossRef] [PubMed]
- J. P. Reithmaier, G. Sek, A. Loffler, C. Hofmann, S. Kuhn, S. Reitzenstein, L. V. Keldysh, V. D. Kulakovskii, T. L. Reinecke, and A. Forchel, "Strong coupling in a single quantum dot-semiconductor microcavity system," Nature 432, 197-200 (2004). [CrossRef] [PubMed]
- E. Peter, P. Senellart, D. Martrou, A. Lemaitre, J. Hours, J. M. Gerard, and J. Bloch, "Exciton-Photon Strong-Coupling Regime for a Single Quantum Dot Embedded in a Microcavity," Phys. Rev. Lett. 95, 067401 (2005). [CrossRef] [PubMed]
- O. Painter, R. K. Lee, A. Scherer, A. Yariv, J. D. O'Brien, P. D. Dapkus, and I. Kim, "Two-Dimensional Photonic Band-Gap Defect Mode Laser," Science 284, 1819-1821 (1999). [CrossRef] [PubMed]
- K. Srinivasan and O. Painter, "Momentum space design of high-Q photonic crystal optical devices", Opt. Express 10, 670-684 (2002). [PubMed]
- J. Vuckovic, M. Loncar, H. Mabuchi, and A. Scherer, "Optimization of the Q factor in photonic crystal microcavities", IEEE J. of Quantum Electron. 38850-856 (2002). [CrossRef]
- Z. Zhang and M. Qiu, "Small-volume waveguide-section high Q microcavities in 2D photonic crystal slabs", Opt. Express 12, 3988-3995 (2004). [CrossRef] [PubMed]
- D. Englund, I. Fushman, and J. Vuckovic, "General recipe for designing photonic crystal cavities," Opt. Express 13, 5961-5975 (2005). [CrossRef] [PubMed]
- S. Noda, K. Tomoda, N. Yamamoto, and A. Chutinan, "Full Three-Dimensional Photonic Bandgap Crystals at Near-Infrared Wavelengths," Science 289, 604-606 (2000). [CrossRef] [PubMed]
- M. Qi, E. Lidorikis, P. T. Rakich, S. G. Johnson, J. D. Joannopoulos, E. P. Ippen, and H. I. Smith, "A three-dimensional optical photonic crystal with designed point defects," Nature 429, 538-542 (2004). [CrossRef] [PubMed]
- S. Ogawa, M. Imada, S. Yoshimoto, M. Okano, and S. Noda, "Control of Ligth Emission by 3D Photonic Crystals," Science 305, 227-229 (2004). [CrossRef] [PubMed]
- M. Okano, A. Chutinan, and S. Noda, "Analysis and design of single-defect cavities in a three-dimensional photonic crystal," Phys. Rev. B 66, 165211 (2002). [CrossRef]
- M. Okano, S. Kako, and S. Noda, "Coupling between a point-defect cavity and a line-defect waveguide in three-dimensional photonic crystal," Phys. Rev. B 68, 235110 (2003). [CrossRef]
- M. Okano, and S. Noda, "Analysis of multimode point-defect cavities in three-dimensional photonic crystals using group theory in frequency and time domains," Phys. Rev. B 70, 125105 (2004). [CrossRef]
- K. M. Ho, C. T. Chan, C. M. Soukoulis, R. Biswas, and M. Sigalas, "Photonic band gaps in three dimensions: new layer-by-layer periodic structures," Solid State Communications 89, 413-416 (1994). [CrossRef]
- S. Kawashima, L. H. Lee, M. Okano, M. Imada, and S. Noda, "Design of donor-type line-defect waveguides in three-dimensional photonic crystals," Opt. Express 13, 9774-9781 (2005). [CrossRef] [PubMed]
- S. Johnson, and J. Joannopoulos, "Block-iterative frequency-domain methods for Maxwell's equations in a planewave basis," Opt. Express 8, 173-190 (2001). [CrossRef] [PubMed]
- A. Farjadpour, D. Roundy, A. Rodriguez, M. Ibanescu, P. Bermel, J. D. Joannopoulos, S. G. Johnson, and G. Burr, "Improving accuracy by subpixel smoothing in FDTD," Opt. Lett. 31, 2972-2974 (2006). [CrossRef] [PubMed]
- J.-P. Berenger, "A Perfectly Matched Layer for the Absorption of Electromagnetic Waves," J. Comput. Phys. 114, 185-200 (1994). [CrossRef]

## Cited By |
Alert me when this paper is cited |

OSA is able to provide readers links to articles that cite this paper by participating in CrossRef's Cited-By Linking service. CrossRef includes content from more than 3000 publishers and societies. In addition to listing OSA journal articles that cite this paper, citing articles from other participating publishers will also be listed.

« Previous Article | Next Article »

OSA is a member of CrossRef.